Ba~3~Li~2~V~2~O~7~Cl~4~, a new vanadate with a channel structure
Reeswinkel, Thomas; Sparta, Karine M.; Roth, Georg; Acta Crystallographica Section C 64 (2008) i38–i40; doi:10.1107/S0108270108002801

data_2016570
_publ_section_title
;
 Ba~3~Li~2~V~2~O~7~Cl~4~, a new vanadate with a channel structure
;
_journal_coeditor_code           SQ3118
_journal_issue                   4
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first              i38
_journal_page_last               i40
_journal_paper_doi               10.1107/S0108270108002801
_journal_volume                  64
_journal_year                    2008
_chemical_formula_iupac          'Ba3 Li2 V2 O7 Cl4'
_chemical_formula_moiety         'O7 V2 , 4Cl , 3Ba , 2Li'
_chemical_formula_sum            'Ba3 Cl4 Li2 O7 V2'
_chemical_formula_weight         781.58
_chemical_name_systematic
;
tribarium dilithium divanadate tetrachloride
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           12
_space_group_name_H-M_alt        'C 1 2/m 1'
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_audit_creation_method           'WinGX routine CIF_UPDATE'
_cell_angle_alpha                90
_cell_angle_beta                 90.592(7)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   16.1215(14)
_cell_length_b                   5.7630(3)
_cell_length_c                   14.3795(13)
_cell_measurement_reflns_used    20576
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      35.23
_cell_measurement_theta_min      2.77
_cell_volume                     1335.90(18)
_computing_cell_refinement       'X-AREA (Stoe & Cie, 2000)'
_computing_data_collection       'X-AREA (Stoe & Cie, 2000)'
_computing_data_reduction        'X-RED (Stoe & Cie, 1996)'
_computing_molecular_graphics    'ATOMS (Dowty, 2000)'
_computing_publication_material  'WinGX (Version 1.70.01; Farrugia, 1999)'
_computing_structure_refinement  'SHELXL97 (Sheldrick, 2008)'
_computing_structure_solution    'SIR2002 (Burla <i>et al.</i>,  2003)'
_diffrn_measured_fraction_theta_full 0.99
_diffrn_measured_fraction_theta_max 0.99
_diffrn_measurement_device       '2-circle goniometer'
_diffrn_measurement_device_type  'Stoe IPDSII'
_diffrn_measurement_method       'Rotation method, \w'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0506
_diffrn_reflns_limit_h_max       25
_diffrn_reflns_limit_h_min       -26
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            22838
_diffrn_reflns_theta_full        34.99
_diffrn_reflns_theta_max         34.99
_diffrn_reflns_theta_min         2.83
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    10.867
_exptl_absorpt_correction_T_max  0.295
_exptl_absorpt_correction_T_min  0.141
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   '(X-SHAPE; Stoe & Cie, 1996)'
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    3.886
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       parallelepiped
_exptl_crystal_F_000             1376
_exptl_crystal_size_max          0.19
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.12
_refine_diff_density_max         1.016
_refine_diff_density_min         -1.267
_refine_ls_extinction_coef       0.00627(10)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL97 (Sheldrick, 2008)'
_refine_ls_goodness_of_fit_ref   1.614
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     106
_refine_ls_number_reflns         3141
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.614
_refine_ls_R_factor_gt           0.024
_refine_ls_shift/su_max          0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     'w = 1/\s^2^(Fo^2^)'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_ref         0.0346
_reflns_number_gt                2763
_reflns_number_total             3141
_reflns_threshold_expression     I>2\s(I)
_cod_data_source_file            sq3118.cif
_cod_data_source_block           I
_cod_database_code               2016570
_cod_database_fobs_code          2016570